Assessment of the Durability Dynamics of High-Performance Concrete Blended with a Fibrous Rice Husk Ash

<jats:p>The present study examines the durability properties of Class 1 (50–75 MPa) high-performance concrete (HPC) blended with rice husk ash (RHA) as a partial replacement of CEM II B-L, 42.5 N. Six HPC mixes were prepared with RHA and used as 5%, 10%, 15%, 20%, 25%, and 30% of CEM II alone and properties are compared with control mix having only CEM II. The binders (CEM II and RHA) were investigated for particle size distribution (PSD), specific surface area (SSA), oxide compositions, mineralogical phases, morphology, and functional groups using advanced techniques of laser PSD, Brunauer–Emmett–Teller (BET), X-ray fluorescence (XRF), X-ray diffraction (XRD), scanning electron microscopy (SEM), and Fourier transform infrared/attenuated total reflection (FTIR/ATR), respectively, to understand their import on HPC. Durability properties, including water absorption, sorptivity, and chemical attack of the HPC samples, were investigated to realise the effect of RHA on the HPC matrix. The findings revealed that the durability properties of RHA-based HPCs exhibited an acceptable range of values consistent with relevant standards. The findings established that self-produced RHA would be beneficial as a cement replacement in HPC. As the RHA is a cost-effective agro-waste, a scalable product of RHA would be a resource for sustainable technology.</jats:p>

section_content: The construction industry contributes significantly to any economy, and its components are vital to advancing socio-economic development goals of shelter, infrastructure, employment, and improved well-being [1]. However, the industry has a long history of negatively affecting the environment and human health. For instance, Rheude et al. [2] attributed high energy consumption, depletion of natural resources, high global anthropogenic CO 2 emissions, waste generation, and air pollution to construction industry activities. Notwithstanding the environmental menaces, Rheude et al. [2] further pointed out that the construction sector is poised to build more urban space in the coming 40 years than in the last 4000 years due to increasing population and urbanisation. The architecture, engineering, and construction (AEC) projects require cement, a major constituent of mortar and concrete cum basic and widely used building material. Adekoya [3] projected Nigeria's local cement production capacity to hit 60 million metric tonnes per annum (MMT/a) by 2022. The report further revealed that key players in Nigeria's cement production, including Dangote Cement PLC, has an installed capacity of 29. 3 MMT/a, followed by Lafarge Africa PLC at 10. 5 MMT/a and BUA Group, which stands at 9 MMT/a with expected plans to increase to 20 MMT/a at the end of 2022. The rise in cement production in Nigeria will continue to increase 0. 870 GtCO 2 emissions recorded in 2015 [4]. Nigeria's high surface area [20]. The addition of RHA brings about denser microstructure and homogeneity in concrete, preventing water and influencing chloride/sulphate ions and chemical agent migration [18]. Consequently, Hu et al. [21] reported a compressive increase of 11. 3% at 28 days of hydration with a 15% replacement ratio with a high reactive RHA. 

From the above, the use of highly reactive RHA with well-graded size distribution and low W/B in a blended cement matrix can achieve a close microstructure and improved durability in HPC. HPC is optimally designed with various fine materials, leading to a very dense microstructure and low permeability. The low transport of moisture and attacking ions impermeability generally improves the durability performances of HPC. Typical durability evaluation of RHA-based cement blend has been determined through chloride and sulphate ion penetration, acid attack, carbonation, shrinkage, sorptivity, porosity, and water absorption resistance tests. Rumman et al. [14] evaluated the chloride permeability resistance of high strength concrete at varied cement contents of 500, 425 and 350 kg/m 3 by RHA contents of 0, 55 and 70 kg/m 3, respectively. The W/B was fixed at 0. 4 and 0. 5 for each mix to propose a new mix design method that incorporates durability as a design factor and RHA as an SCM. Their results revealed that up to 20% RHA content, chloride permeability was reduced to approximately 63%. Hossain et al. [7] investigated the water absorption and sorptivity of a high strength mortar containing RHA as an SCM. A mix ratio of 1:3, with W/B of 0. 4 and 0. 5 at 5-20% cement replacement of five steps, was adopted. The hardened mortar samples were subjected to two different curing schemes (standard and high-temperature curing) for 1, 7, and 28 days. The water absorption and sorptivity test results revealed that RHA blended mortar with a high-temperature curing method showed an overall decline in water absorption and sorptivity. 

Sahoo et al. [18] assessed the durability properties (water permeability, sorptivity, porosity, chloride permeability, carbonation resistance, and weight loss due to acid attack) of a normal strength concrete blended with RHA. At 15% RHA content cured for 28 and 60 days, sulphur acid attack reduced by 7% whereas the water permeability reduced by 15% at 90 days. The carbonation resistance result showed approximately 0. 13 cm/day 0. 5 in the magnitude of co-efficient of carbonation at 90 days. Chloride ion penetration recorded a reduction of approximately 15% at 10% RHA content, whereas 15% RHA content increased to 26. 1%. Similarly, De Silva et al. [19] examined the effect of waste RHA residual ash from rice husk fueled brick kilns on the durability properties of a plastering mortar. With 550 kg/m 3 cement content, RHA was varied from 5-10% in five steps. Their finding showed a reduction of 54% and 70% in sulphate exposure for 5% and 10% RHA content. Weight loss in an alkaline environment reduced from 3. 13% to 2. 4% in 10-15% RHA content. Swaminathan et al. [22] investigated the influence of a ternary mix of Portland cement, metakaolin, and RHA on the durability properties of an M60 grade HPC. Their results revealed that the durability dimensions of water absorption, sorptivity, porosity, and permeability penetration improved due to RHA's presence in the mixture. Finally, Wang et al. [15], in their review of RHA performance on cementbased materials under various W/B, pointed out within 10-25% RHA content, chloride penetration resistance is optimised, carbonation resistance best improved at 20%, and shrinkage resistance optimisation stands at approximately 10-20% cement replacement. Wang et al. [15] placed sulphate resistance optimisation at 40 and 50% RHA content in the cementitious material. Generally, the authors noted that tested concrete and mortar samples' durability and mechanical properties improved within 10% and 20% of RHA content. 

RHA has attracted a lot of research on the strength properties of normal strength concrete and mortar. However, few studies are available on durability dimensions of HPC, especially in developing countries like Nigeria. Hence this study investigates the durability properties of water absorption, sorptivity, and chemical attack of a fibrous RHA blended in HPC mixtures. The aim is to understand the feasibility of incorporating a controlled incinerated RHA into an HPC matrix in fulfilling its long-term durability properties. The information will be relevant for further RHA use in sustainable construction materials and the industry's growth.
section_name: Introduction

section_name: Materials and Methods

section_content: Portland-limestone cement (CEM II B-L, 42. 5 N) conforming to BS EN 197-1 [23] and NIS 444-1 [24] is used as the main binder in the current experiment. Here, RHA is used as a replacement for CEM II and produced in a controlled incinerator at 700 • C for 1 h in an electric furnace and pulverised using a grinding mill at Laboratory of Nigeria Cereals Research Institute, Baddegi, near Bida in Niger State, Nigeria. The workability of the HPC samples was improved using Masterglenium Sky 504-a polycarboxylic ether polymerbased superplasticiser supplied by BASF Limited (Lagos, Nigeria) and used within the manufacturer's best specification of ≤2% weight of binder (b wob ). The internal curing agent of superabsorbent polymers (SAP) tagged "FLOSET 27CC ≥ 300 µm" was added at fixed content of 0. 3% by b wob. The particle size distribution (PSD) and specific surface area of the binders were measured via the laser PSD (Malvern Mastersizer 3000, Worcestershire, UK) and Brunauer-Emmett-Teller, BET (Nova Station B Quantachrome Instrument, Boynton Beach, FL, USA) methods. Oxide compositions, mineralogical phases, and the morphology of the binders were analysed using X-ray fluorescence, XRF (Bruker AXS S4, Explorer, Karlsruhe, Germany), X-ray diffraction, XRD (Rigaku Miniflex 600, Washington, DC, USA), and scanning electron microscopy, SEM (Phenom ProX, PhenomWorld, Eindhoven, The Netherlands) techniques, respectively. The functional groups were investigated with Fourier transform infrared/attenuated total reflection, FTIR/ATR (Cary 630, Agilent Technologies, Penang, Malaysia).
section_name: Materials 2.1.1. Binders

section_content: Dry-conditioned river sand with a nearest particle size of 300 µm was used as fine aggregate in the experimental study [9, 25]. Similarly, a 13. 50 mm crushed granite stone retained on a 9. 50 mm sieve size served as a coarse aggregate [9, 26]. The coarse aggregate was washed to remove compromising materials and implemented at saturated surface dry condition. The mechanical and physical properties of the aggregates were also analysed for PSD (standard sieves), specific gravity, water absorption, aggregate crushing, and impact values.
section_name: Aggregates

section_content: Portable water devoid of any toxic and floating materials and complying with BS EN 1008 [27] was used to prepare the HPCs.
section_name: Water

section_content: In line with the goal of this experimental work, seven variant mixtures inclusive of a control mix were designed. The control mix was designed for 28-day Class 1 (50-75 MPa) HPC having characteristic cube strength of 67 MPa, following the British method of HPC design. The other six HPCs mixtures were designed by replacing 5%, 10%, 15%, 20%, 25%, and 30% with RHA. A fixed 0. 3 and 0. 3% for W/B and SAP content by b wob was maintained, respectively, and superplasticiser content of 1. 5% b wob was added for all the HPC mixtures to improve the workability. Added water of 12. 5 g/g of SAP was furnished for the SAP permeability on the basis of the work of Olawuyi [28]. Each constituent of HPC was measured by weight (kg/m 3 ), and hence, the RHA additive was taken to be by weight of the binder. The HPC assemblies were labelled with the name "RHAC" and the replacement level. For instance, the HPC having RHA with 5% replacement was implied as RHAC-5. The details of the number of materials computed for all the seven HPC mixtures and their mix identifications are presented in Table 1.
section_name: HPC Mix Design

section_content: Having obtained the required materials, they were mixed in a 50 litre pan-mixer to obtain a uniform workable mix. First, the fine aggregate followed by the binders were mixed in the pan-mixer for 1 min. Next, dry SAP particles were added, and all the fine contents were mixed for another 30 s. After that, the coarse aggregate was introduced, and mixing was maintained for 1 min before water previously mixed with superplasticiser was added. Finally, the mixing was sustained for an additional 3 min to obtain a harmonised workable fresh HPC mix, as proposed in the literature [28, 29]. The fresh HPC was later undertaken for workability test via the slump flow. After fulfilling the workability standards fixed at 450 mm-600 mm flow value [9], the fresh HPC was poured into various previously oiled moulds of specified sizes. The specimens for the various tests were cast in two layers on a vibrating table. The cast samples were then protected in the laboratory with thick vapour barriers and allowed to harden for 24 h before demoulding, and they were then left to cure in a water tank at 20 ± 3 • C until the required curing ages (7, 28, 56 and 90, days respectively) before testing in accordance to standards [30] [31] [32] [33].
section_name: Production of Fresh HPC, Sample Casting, and Curing

section_content: The details concerning the specimen type, testing age, and standard followed for each test developed in the experimental study is provided in Table 2. The water absorption was examined on 100 mm size cubes following EN, B. 1097-6 [31]. The HPC samples were initially immersed in water for 28, 56, and 90 days with their weight obtained and tagged M wet. After that, the samples were oven-dried at 110 ± 5 • C in triplicates pending a stable weight for 24 h. The dry samples were left to cool and then measured and recorded, denoted as M dry. The water absorption value was analysed by subtracting the dry samples' weight from the saturated sample, dividing the result by the dry sample's weight, and multiplying by 100. Mathematically, water absorption, WA, value can be expressed as in Equation ( 1 ):

Mwet -Mdry Mdry × 100 (1) where WA (%) is the water absorption value; M wet is the wet sample's weight; and M dry is the dry sample's weight. 

In the same vein, for investigating the water sorptivity test, water was allowed via a face of the Ø100 × 50 mm disc specimen under capillary action in line with ASTM C1585-04 [30]. First, the disc samples in triplicates were oven-dried at 110 ± 5 • C until reaching a fixed weight for 24 h. The discs were weighed again before dipping in approximately 30 mm of water. Samples were kept there for approximately 7 h, and data were recorded after 5, 10, 15, 30, 60, 120, and 180 min. The samples were then removed and weighed again to observe the amount of absorbed water. Equation (2) shows the results: I = S. t 0. 5 (2)

where I represents the cumulative ingress of water in mm, S is the sorptivity coefficient, and t, min is the sample's immersion time in the water. The mass of water absorbed into the specimen was converted into the volume. The volume of water plotted against the square root of time gives a straight line. The sorptivity coefficient was calculated by measuring the slope of this straight line. A best-fitted line was then computed using a regression analysis of data points for every HPC mix. The slope of the best-fitted line was the rate of absorption for that mixture. The chemical attack of the HPCs was evaluated by immersing the specimen in 5% hydrochloric acid (HCl), 5% sodium sulphate (Na 2 SO 4 ), and 5% calcium chloride (CaCl 2 ) solutions, respectively. The pH of the acidic, chloride, and sulphate environments were studied during the testing cycle. The solutions were renewed every 30 days after checking the pH of the solutions. The specimens were removed at 7, 28, 56, and 90 days after being exposed to acid, chloride, and sulphate solutions and washed with water. The effects of acid, chloride, and sulphate attack were evaluated based on compressive strength assessment. The compressive strength followed BS EN 12390-3 [32] and RILEM Technical Recommendation TC14-CPC 4 [34]. The HPC cubes were investigated using the Model YES-2000 digitised Materials Testing Machine (Eccles Technical Engineering Ltd., England, UK) with a 2000 kN maximum loading capacity.
section_name: Testing Procedures

section_name: Results

section_name: Characterisation of Binders

section_content: Figure 1 shows that 90% (D 90 ) of CEM II and RHA particles are smaller than 4000 and 3900 nm, respectively. The median particle size, D 50 of CEM II and RHA is 48. 8 and 3200 nm, respectively. Furthermore, the particle size below 10% (D 10 ) falls within 4. 88 and 160 nm, respectively, for the same samples. From Table 3, the SSA measured via the MultiPoint BET model showed 8. 182 × 10 2 and 4. 649 × 10 2 m 2 /g for CEM II and RHA, respectively. The pore diameter of the binders analysed through the DA BET mode indicated corresponding values of 2. 92 and 1. 52 nm for CEM II and RHA samples. Based on these values, CEM II particles are finer than RHA particle size with a surface area close to each other. The physical properties of CEM II is available at [11]. Comparing the two binder's DA BET analysis, the RHA sample has a lower pore size diameter, conforming to macro-mesoporous material [35] and the SSA conforming to Kwan and Wong [36]. The results in Table 4 inform the choice of the SCM having functional oxides (SiO2 + Al2O3 + Fe2O3) of 82. 62% and conform to ASTM Standard C 618 [37]. The chemical composition of CEM II is available at [11] study. The total amount of silica, alumina, and iron oxide required for mineral admixture's amorphousness is rated to be above 70%. This standard only guides mineral admixtures' potential reactivity [38]. RHA here contains 80% SiO2, 1. 8% Al2O3, 0. 8% Fe2O3, and 0. 8% CaO. It can be noticed that the Fe2O3 of CEM II (3. 19) was greater than the RHA (0. 79), which could be responsible for the higher specific gravity and density. However, the oxide percentage of RHA depends on the type, source, origin, and calcination systems. CEM II contains CaO and SiO2 of approximately 57% and 15%, respectively. The CaO and SiO2 oxide percentage values obtained here are below the limits of 60-67% (CaO) and 17-25% (SiO2), respectively, recommended by Newman and Choo [39] for 42. 5 N cement class. There exists a 9. 18% difference in the useful chemical oxides found in the RHA used in the present study and those reviewed by Mosaberpanah and Umar [40]. For example, they found the average useful oxides of SiO2, Al2O2, and Fe2O2 in RHA in India, Vietnam, Malaysia, Brazil, and the USA to be 90. 98%. Therefore, RHA's chemical oxide composition generally conforms to class N of ASTM C 618 [37] minimum requirements for possible pozzolans. [11] study. The total amount of silica, alumina, and iron oxide required for mineral admixture's amorphousness is rated to be above 70%. This standard only guides mineral admixtures' potential reactivity [38]. RHA here contains 80% SiO 2, 1. 8% Al 2 O 3, 0. 8% Fe 2 O 3, and 0. 8% CaO. It can be noticed that the Fe 2 O 3 of CEM II (3. 19) was greater than the RHA (0. 79), which could be responsible for the higher specific gravity and density. However, the oxide percentage of RHA depends on the type, source, origin, and calcination systems. CEM II contains CaO and SiO 2 of approximately 57% and 15%, respectively. The CaO and SiO 2 oxide percentage values obtained here are below the limits of 60-67% (CaO) and 17-25% (SiO 2 ), respectively, recommended by Newman and Choo [39] for 42. 5 N cement class. There exists a 9. 18% difference in the useful chemical oxides found in the RHA used in the present study and those reviewed by Mosaberpanah and Umar [40]. For example, they found the average useful oxides of SiO 2, Al 2 O 2, and Fe 2 O 2 in RHA in India, Vietnam, Malaysia, Brazil, and the USA to be 90. 98%. Therefore, RHA's chemical oxide composition generally conforms to class N of ASTM C 618 [37] minimum requirements for possible pozzolans. Figure 2 shows the diffractograms of CEM II. There is a reflection of quartz (SiO 2 ), wollastonite (Ca Si O 3 ), garnet (Ca, Fe, Mg) O Al, Fe. . . )), osumilite (K-Na-Ca-Mg-Fe-Al-Si), and calcite (CaCO 3 ). Osumilite mineral takes the most dominant phase of 19%, followed by garnet with 16% phase representation by weight. The presence of quartz mineral, which is mostly not affected by heat treatment [41], is seen in the diffractograms phase spectra at 6%. Wollastonite and calcite minerals were visible at 4% and 3% weight content, respectively. The two major chemical oxide components (calcium and silica oxides) presents osumilite as having good potential for cement production [42]. The result is coherent with the XRF data of CEM II studied here. Figure 3 shows the phase pattern view of the calcined RHA highlighting quartz (SiO 2 ), apatite (Ca 5 (F. Cl) P 3 O 12 ), englishite (K 3 Na 2 Ca 10 Al 15 [PO 4 ]), and garnet 3(Ca, Fe, Mg) O. Al, Fe) as the mineral contents of the studied sample. The spectrum peak pattern can be described as apatite (13%) as the most dominant mineral present in the calcined RHA, followed by garnet and englishite with 4% mineral deposits. Quartz (SiO 2 ) has the lowest mineral peak phase of 3%. The XRD examination confirms the SiO 2 chemical oxide composition dominance in the XRF analysis. Thus, the result further revealed that calcining RHA up to 700 • C could produce an amorphous material (76%) suitable for concrete improvement.
section_name: Physical Properties of Binders

section_content: The SEM images of the two binding materials put together (CEM II and RHA) are shown in Figures 4 and 5, respectively. Figure 4 projects the SEM images of CEM II used in this study when viewed at 100 µm and 200 µm magnification settings. The images are irregular, close to angular in shape, and interconnected. Micro-air space (dark spots, C) detaches the grains, prompting the specific grains to be recognised. The CEM II SEM image also indicated two grey band readings for particles (i. e., light grey, A and dark grey, B) portraying C 3 S (alite) and C 2 S (belite), respectively. The white spots represent the Fe + or Al + in C 3 S or C 4 AF. The results from the morphology of CEM II is consistent with Joshua et al. [43] SEM findings on major cement brands in Nigeria. The SEM image of the whitish RHA powder (Figure 5 ) particle at the same 100 µm and 200 µm magnifications also showed a smooth broad surface and slightly irregular shaped particles. The SEM image manifested dark grey and light grey irregular shapes indicated as G and H, respectively, in Figure 5.
section_name: Morphology of Binders

section_content: Figure 6 shows the FTIR/ATR transmittance spectra of anhydrite CEM II, 42. 5 N. The IR bands at 712, 872, 910, 1111, 1420, 1685-1793, and 3381-3422 cm -1 emerged as a result of v 4 -stretching of carbonate, v 2 -out of plane vibration CO 3 2-, S-O stretching of SO 4 2-, v 3 -asymmetric stretching of CO 3 2-, bending mode of water, presence of CaCO 3, and stretching of OH band, respectively [44]. The weak peak of 3422 cm -1 in the high zone highlights OH stretching of Ca(OH) 2, indicating a poor portlandite formation. The close absorption bands between 3381 and 3422 cm -1 in the FTIR spectra's peak region revealed that CEM II contains fewer water molecules. Figure 7 shows the IR spectra obtained from the calcined RHA characterised in this work. Peak identification was performed based on studies by Srivastava et al. [45] and Totlani et al. [46]. According to the authors, at 3709 and 2920 cm -1 bands, both free and hydrogen-bonded OH groups and Si-OH group on the adsorbent surface exist. The stretching arises due to the silanol groups (Si-OH) and adsorbed water on the surface. The author pointed out that CO groups' transmittance of vibration in lactones occurs at 1050-1300 cm -1 bands. The presence of Si-H is usually at 793 and 469 cm -1 bands. As shown in Figure 7, there appear to be steady transmittances of Si-OH groups, Si-CH-CH 2 stretch, and aromatic compounds (H-C), respectively, from 3700 to 1300 cm -1 bands. The peak of the 1066 cm -1 band may be attributed to CO groups' vibration transmittance in lactones. Finally, the presence of Si-H is seen at the transmittance peak of 793 cm -1 bands. All the spectra conform to those found in the literature [45] [46] [47].
section_name: FTIR/ATR of Binders

section_content: The PSD plot in Figure 8 shows that the fine aggregate sample is medium sand of Shetty [48] group, whereas the coarse aggregate used for the study is uniformly graded stone. The physical characteristics of the fine and coarse aggregate are tabulated in Table 5 available in [11] study. The fine aggregate recorded fineness modulus (FM) of 2. 87; coefficient of uniformity (Cu) of 2. 39; coefficient of curvature (Cc) of 0. 94; specific gravity (SG) of 2. 65; and water absorption = 1. 2% in the physical properties' tests. In the same vein, the coarse aggregate analysed for the study had a specific gravity of 2. 7, water absorption of 1. 05%, aggregate crushing, and impact values of 28% and 11%. These findings were expected and reinforced the usefulness of sieving out finer particles of the river sand with 300 µm sieves and washing coarse aggregate to minimise the dust content, which complied with requirements in the literature [25, 49]. There are similarities in fineness modulus (2. 87) and the specific gravity of sand (2. 79) between the present study and those described by Mermerdaş et al. [50]. The particle size distributions of the fine and coarse aggregates in the present study are consistent with the description of aggregates used in Zhou et al. [51].
section_name: Characterisation of Aggregates

section_content: The plot showing the observed slump flow values for the control and mixes containing RHA at various percentage replacements is presented in Figure 9. It can be observed from the figure that the slump flow for HPCs blended with RHA recorded increases of 4. 81%, 8. 65%, and 1. 92% for RHAC-5, RHAC-10, and RHAC-15 mixtures, respectively, when compared to the control mixture. Additionally, RHAC-20, RHAC-25, and RHAC-30 had a reduced slump flow of 11. 53%, 23. 08%, and 39. 42%. This phenomenon may be because the ground RHA had a particle size distribution similar to CEM II, so there was a high-water demand effect. The results from RHAC-5 to RHAC-20 are in conformance to the slump flow range of 450 mm-600 mm, as recommended by Neville [9]. An important issue emerging from these results is that HPC containing RHA as a cement substitute requires more water than the control mix to develop similar workability. The average test results for the RHA blended HPCs' water absorption at 28, 56, and 90 days are illustrated in Figure 10. The water absorption varied in the ranges of 1. 27-3. 88% for 28 days, 2. 80-5. 62% for 56 days, and 2. 50-5. 13% for 90 days. Most findings are inconsonant with the acceptable range of water absorption for HPC, as pointed out by ASTM C 642 [52]. The standard specifies high-quality concrete to have water absorption in the range of 2-5%. Thomas [53] averred that low range water absorption in RHA based concrete is due to the limited pore connectivity and reduced porosity of the concretes. However, the water absorption of RHAC-30 was higher than the specified standard at 56 and 90 days, respectively. This increase may be related to the apparent porosity features of RHA. Once the apparent porosity of RHA based HPC increases, it is anticipated that water absorption will increase. The increase in water absorption of RHA based concrete is reported by Olutoge and Adesina [54] while relating the phenomenon to the hygroscopic nature of RHA material. As can be seen, there was a slight improvement at 90 day observations. All the RHA blended mixtures showed improvement at 90 days curing compared to the 56 days observation. The water absorption of the HPCs increased with a greater RHA content, as evident in all the RHA based HPCs at curing days. The control sample attained the lowest level of water absorption in all curing days. Usually, water absorption is affected by the water to cement ratio, the paste's content and volume in the concrete mix. In this light, water absorption will increase when the volume content of RHA increases.
section_name: Workability (Slump Flow)

section_content: The variations of water absorption by capillary pressure in relation to time passed are depicted in Figures 11 12 13. The absorption rate (sorptivity coefficient) graphs for RHA blended HPCs were computed between the change in weight per unit area over the unit weight of water and the period's square root (minutes). the effects of blended RHA on the water sorptivity of HPC at 28, 56, and 90 days. The capillary water action decreased as the curing days progressed for the control mix. The RHA blended mixtures water sorptivity fluctuated due to the RHA's pore structure, particle size distribution, and specific surface area affecting their microstructure and cement hydration. A 28-day CEM II had the highest water capillary ingress of approximately 5. 5-6. 4 mm over the 180 min inspection time. The RHA blended HPCs had an average water sorptivity of 2. 93 mm, higher than that of the control mix (1 mm). A similar trend continued for 90 days; the average water ingress was computed to be 2. 96 mm for the MCC blended HPCs. 

The control at the same age had a lower water absorption value (0. 44 mm) than the RHA blended mix. The 10% cement replacements at 28 and 56 days gave the best water sorptivity values, supporting the mechanical properties results. These inconsistencies may be due to RHA's micro, macro, and mesoporous structure, which influenced its pozzolanic activity and specific surface area. The RHA blended matrix performed slightly more poorly in water sorptivity compared to the control mix. A reverse behaviour could be expected regarding a higher specific surface area, pore structure, and pore size distribution given in Table 4. The binary mix of cement (slightly finer than RHA) and calcined RHA is expected to yield a higher packing density in a granular mixture [55]. Therefore, this study's findings situate well with Vieira et al. [35], who studied the effects of various particle size distribution and replacement contents of RHA on the compressive strength of HPC. 

Table 6 reports the correlation coefficient of RHA modified HPC at 28, 56, and 90 days. The control mix showed a near relationship between the rate of absorption and the square root of time at 28 days with a computed coefficient of correlation (R 2 = 0. 83), whereas 56 and 90 days had close to insignificant coefficients of correlation (R 2 = 0. 98 and 0. 94, respectively). This finding is an indication of further hydration tendencies of the tested samples as curing days increased. The correlation coefficients were R 2 = 0. 98, 0. 96, 0. 99; 0. 88, 0. 98, 0. 94; 0. 97, 0. 95, 0. 99; 0. 98, 0. 88, 0. 96; 0. 95, 0. 96, 0. 99 and 0. 92, 0. 98, 0. 95, respectively, for RHAC-5, RHACC-10, RHACC-15, RHACC-20, RHACC-25, and RHACC-30, respectively. These data must be interpreted with caution because of their close relationships. ASTM C 1585 [30] pointed out that "If the data between 1 min and 6 h do not follow a linear relationship (a correlation coefficient of less than 0. 98) and show a systematic curvature, the initial rate of absorption cannot be determined". The correlation coefficient of RHAC-5 was near significant in 28 and 56 days and significant at 90 days. RHAC-10 recorded a moderate significant difference at 28 days. MCCC-15 to MCCC-30 mixtures highlighted varied insignificant differences in the measured coefficient of correlation across the 28, 56, and 90 day tests. There are several possible explanations for this result. For example, Le and Ludwig [55] found that adding calcined RHA in cement matrix increases cement hydration due to their nucleation and dilution effects coupled with higher packing density in granular mixtures. From the figures, the control exhibited a compressive strength variation between 2. 20 and 14. 02% after 7, 28, 56, and 90 days of acid, sulphate, and chlorine solutions curing and compared with water immersion curing. There is a decrease in percentage compressive strength loss as the curing ages increase in the HPC control sample. At all the mix types, the chlorine environment showed a relatively high impact on the tested sample compressive strength. The RHAC-5 mixture exhibited a compressive strength drop between 10. 59 and 22. 02% after 7, 28, 56, and 90 days of acid, sulphate, and chlorine curing. Whereas for other mixes (RHAC-10 to RHAC-30), the compressive strength drops between water and other chemical environments curing obtained was in the range of 2. 83 to 9. 81% at 7, 28, 56, and 90 days. HPCs containing RHA tend to show superior compressive strength reduction in the studied chemical environments. Analysing the results, it can be inferred that mesoporous RHA particles dominated the void areas in HPC, leading to reduced acid and sulphate attacks and chlorine migration into the matrix. The findings here complied with Thomas [53] on optimised 15-20% cement replacement with RHA capability of reducing acid attack and chloride penetration in concrete.
section_name: Sorptivity of HPCs

section_content: The current paper examines the durability dimensions of water absorption, sorptivity, and chemical attack of an HPC blended with an agricultural by-product of RHA. CEM II was replaced at 5%, 10%, 15%, 20%, 25%, and 30% with RHA, having a constant 0. 3 W/B and a 0. 3% by weight of binder content of SAP in the HPC mixture. The plastic property of the mixture was evaluated using the slump flow test, and the results were compared with the propositions of Neville [9]. The following inferences are drawn from the research.
section_name: Conclusions

section_content: The RHAC-5 to RHAC-20 are the only RHA based HPC that conformed to the slump flow range of 450 mm to 600 mm.
section_name: •

section_name: Acknowledgments:

section_content: The authors extend their appreciation to the suppliers of the superplasticiser-Masterglenium Sky 504-BASF Limited, West Africa; the Superabsorbent Polymers (SAP)-SNF Floerger-ZAC de Milieux, France, and 100 mm cube metal moulds-the Nigerian Building and Road Research Institute (NBRRI), Ota.
section_name: Acknowledgments:

section_content: Funding: This paper received no external funding, and the APC was funded by Covenant University Center for Research, Innovation and Discovery (CUCRID).

section_name: •

section_content: The water absorption values obtained in RHA based HPCs are within the 2-5% acceptable range of water absorption for HPC, conforming to ASTM C 642 [52].
section_name: •

section_content: The sorptivity correlation coefficients are less than or equal to 0. 98 for RHA blended HPCs, conforming to ASTM C 1585-04 [30].
section_name: •

section_content: Mesoporous RHA particles dominated the void areas in HPC, leading to reduced acid and sulphate attacks and chlorine migration into the HPC matrix.
section_name: •

section_content: The chlorine environment at all the mix types showed a relatively high impact on the tested samples' compressive strengths.
section_name: •

section_content: These findings validated that that locally produced RHA would have potential as a cement replacement in HPC.
section_name: •

section_content: Subsequently, the RHA is an economical agro-waste; a scalable product of RHA would be a resource to sustainable technology.
section_name: •

section_content: The authors declare no conflict of interest.
section_name: Conflicts of Interest: